Solar Energy R&D
in the European Community
Series E Volume 7
Energy from Biomass
The Traditional and Industrial Methods
Springer-Science+Business Media, B.V.
library of Congress Cataloging in Publication Data
Handbook of charcoal making.
(Solar Energy R&D in the European Community. Series E, Energy from
biomass; v. 7) (EUR; 9590)
Inc1udes bibliographie s.
I. Charcoal. I. Commission of the European Communities.
II. Title. III. Series: Solar energy R & D in the European Community.
Series E, Energy from biomass; v . 7. IV. Series: EUR; 9590 .
TP33l.E45 1985 662 '.74 84-27630
ISBN 978-90-481-8411-8 ISBN 978-94-017-0450-2 (eBook)
Publication arrangements by
Commission of the European Communities
Directorate-General Information Market and Innovation, Luxembourg
<0 1985 Springer Science+Business Media Oordrecht
Originally publi shed by ECSC, EEC, EAEC, Brussels and Luxernbourg in 1985.
Softcover reprint ofthe hardcover Ist edition 1985
Neither the Commission of the European Communities nor any person acting on behalf of the
Commission is responsible for the use which might be made of the following information.
All Rights Reserved
No part of the material protected by this copyright notice may be reproduced or utilized
in any form or by any means, electronic or mechanical, inc1uding photocopying,
recording or by any information storage and retrieval system,
without written permission from the copyright owner.
We are happy to introduce the Handbook of Charcoal-Making, a
comprehensive survey written by a competent expert with international
experience. The book was prepared by the Commission of the European
Communities in the frame of its R + D programme on biomass.
In the European Community today the biomass option is only little
developed: a huge resource is waiting for use .
Actually, there is ample scope for biomass utilisation as it bears
promise in some of the vital sectors of modern society. Development of
indigenous and renewable energy sources, creation of new employment,
recycling of wastes and improvement of the environment, restructuring of
European agriculture, development of the Third World, they are all
It is important to note that the exploitation of the biomass resource is
largely related to its conversion into a marketable product . However,
as many of the conversion technologies are not yet well established or
need improvement, R + D is more than ever the critical pathway to get
access to the benefits of biomass utilisation .
In the European Communities I R + D programme, thermal conversion of
biomass is developed with priority. Gasification as well as pyrolysis
development projects are being supported by the Commission in European
industry and universities.
Pyrolysis is particularly attractive because the conversion products
charcoal and pyrolytic oil are very convenient in use, technologies are
relatively simple and projected pay-back times favourable.
Charcoal making is just the simplest and oldest form of pyrolysis.
Charcoal is already a market product and plays an important role in the
energy consumption structures of most developing countries.
As modern literature on charcoal is' scarce, this book will first of all
serve the purpose of a review book of the state-of-the-art.
Furthermore, it is essential as a reference book for future R + D in
view of technical improvements and new processes of charcoal making and
pyrolysis in general.
I take this opportunity to thank Dr. Walter Emrich for having accepted
the Commission's invitation to write this book. I also thank
Mr. L. Crossby and Mr. J .F. Molle for reviewing the manuscript.
I wish the book great success.
Dr. W. 'Palz
R + D Programme Biomass
Commission of the European Communities
LIST OF ILLUSTRATIONS
AND FUNDAMENTALS OF THE CHARCOAL PROCESS
Charcoal-Making from the Beginning until
the Present Day
Theory of the Carbonization Process
Heating Systems for Charcoal Plants
Properties of Carbonization Products
TRADITIONAL METHODS OF THE SMALLHOLDER CHARCOAL-MAKER
Charcoal Pits and Earthmound Kilns
The Charcoal Pit
The Earthmound Kiln
The Earthmound Kiln with Chimney
The Earthmound Kiln with Tar Recovery
Charcoal-Making with Portable and
2.2.1 The Tongan Oil Drum Kiln 39
2.2.2 The Philippines Kiln 42
2.2.3 The Black Rock Forest Kiln 45
2.2.4 Sectional Metal Kilns 48
2.2.5 The Carborion Kiln 54
2.3 Concrete and Brick Kilns 56
2.3.1 The Missouri Kiln 60
2.3.2 Cinder Block Kilns 66
2.3.3 The Schwartz and Ottelinska Furnaces 74
2.3.4 The Brazilian Beehive Brick Kiln 77
2.3.5 The Argentine Kilns 88
2.4 Kiln Designs for Waste Conversion 99
2.4.1 The Carbo-Gas Retort 101
CONCEPTS AND TECHNOLOGY FOR THE INDUSTRIAL
3.1 Equipment for Charcoal Plants with
3.1.1 The Forerunners of Modern Charcoal
The Wagon Retort
The Reichert Retort Process
The French SIFIC Process
Charcoal Technology for The Carbonization
Generalized Flow Diagram
The Multiple Hearth Furnace
The Fluid Bed Carbonizer
The Vertical Flow Converter
The Enerco Mobile Pyrolyser (Model 24)
TECHNIQUES FOR RECOVERING COMMERCIAL PRODUCTS FROM
PYROL YSIS OIL 148
4.1 Pyrolysis Oil Recovery 149
4.2 Crude Acetic Acid and Acetone Recovery 150
4.3 Recovery of Methanol (Wood Spirit) 152
4.4 Processing of Charcoal Tar 154
4.5 Concluding Remarks 159
RAW MATERIALS SUPPLY 162
5.1 Supply from Fuelwood Plantations 165
5.2 Agricultural Resources 166
5.3 Transport and Preparation of Raw Materials 168
5.3 .1 Key Factors in Wood Supply 169
MARKETS FOR CHARCOAL AND CHARCOAL BY-PRODUCTS
Charcoal as Household Fuel
Charcoal as Fuel for Industry
Charcoal in Metal Extraction
Synopsis of Industrial Active Carbon Markets
Speciality Markets for Charcoal
Charcoal for Producer Gas
Synopsis of Major Uses of Charcoal and
Charcoal Costs and Fuel Prices
Packing and Shipment for Export/Market
- ix -
PLANNING A CHARCOAL VENTURE AND SELECTION OF EQUIPMENT 208
7.1 Planning of Projects 211
7.2 Selection of Charcoal Equipment 214
7.3 Conclusions 220
CHARCOAL BRIQUETTES AND ACTIVATED CHARCOAL
8.1 The Briquetting Process 223
8.1.1 Simple Briquetting Equipment 227
8.2 The Activated Charcoal Process 228
SAFETY PRECAUTIONS AND ENVIRONMENTAL CONSIDERATIONS 234
9.1 Safety in Charcoal Operations 234
9.2 Safety Devices and Equipment 236
9.3 General Safeguarding of Charcoal Plants 237
9.4 Precautions for Charcoal Storage 238
9.5 Environmental Considerations for the
CHARCOAL LABORATORY WORK 243
10.1 Analysis 244
10.2 Bench-Scale Carbonization Tests 251
Case Studies 255
Energy Distribution Diagram 265
Addresses of Consultants, Institutes,
and Equipment Suppliers 268
Conversion Tables 275
- x -
LIST OF ILLUSTRATIONS
Temperature diagrams of dry distillation 6
Temperature distribution diagram (continuous
Heating systems 9
Classification of charcoal processes 10
Carbon content and higher heating value.
Moisture content and net heating value 23
A charcoal pit 26
A small earthmound kiln 28
A large earthmound kiln with centre firing 31
An earthmound kiln with chimney 34
An earthmound kiln with pyrolysis oil
The Tongan oil drum kiln 40
The Philippines oil drum kiln 43
The Black Rock Forest kiln 46
Handling the kiln with a derrick 46
A battery of four Black Rock Forest kilns
in operation 47
A portable metal kiln 50
Air inlet channels at the bottom of a
portable metal kiln with wood grate 50
The Carborion kiln 55
The Missouri charcoal kiln 58
Plan and elevation of the Missouri kiln 59
A cinder-block charcoal kiln 67
Typical masonry units for block-type
charcoal kilns 70
Detail of the thermocouple assembly on the
lengthwise centreline of a cinder-block kiln 72
The Schwartz charcoal furnace 75
The Ottelinska furnace 75
26 Improving the Schwarti system by installing
27 The Brazilian beehive brick kiln 79
28 The slope-type beehive brick kiln 80
29 Beehive fire brick kiln with external heating 81
30 A charcoal production centre 86
31 Half orange kiln with straight jacket 91
32 Carbo-Gas retort (twin unit) 100
33 Carbo-Gas retort plant with charcoal gas
recovery for commercial use 100
34 The Carbo furnace 111
35 The Bosnic charcoal plant 113
36 A smaller Bosnic plant with interchangeable
37 The wagon retort plant 118
38 The Reichert retort process 122
39 The French SIFIC retort process 124
40 Side view of the CISR Lambiotte plant 127
41 Generalized flow diagram of the rapid
pyrolysis process 131
42 Cross-section of a multiple hearth furnace 134
43 The fluid bed carbonizer. Generalized diagram 137
44 The vertical flow converter 140
45 The ENERCO model 24 pyrolyser 145
46 A charcoal plant with pyrolysis oil refinery 153
47 Recovery of commercial products from
pyrolytic tar 155
48 A wood dryer for continuous operation 174
49 The integrated carbonization concept with
four carbonizers 212
50 Simple charcoal briquetting press 226
51 Activated carbon plant for manufacturing
of pellets or granular active carbon 231
52 Apparatus for bench-scale dry distillation 252
53 The energy distribution diagram 266
1 Small earthmound kiln in Ghana one hour
after lighting. 30
2 Discharging charcoal from same kiln
two days later. 30
3 A Missouri kiln. The shell is dangerously
cracked as a result of faulty operation. 63
4 Side view of kiln with two smoke pipes and
air inlet holes at the bottom 63
5 Charging the beehive brick kiln . 85
6 A Brazilian beehive brick kiln in full
ope ration. 85
7 The Argentine half-orange kiln. The operator
is closing the gate after charging the kiln. 90
8 Small half orange kiln (7 m3) 92
9 Charcoal trainees in Kenya constructing
a half orange kiln with straight jacket. 92
10 Charcoal trainees igniting the kiln with
a shovelful of ,glowing charcoal. 93
11 Charcoal train~e brushes over leaks . 93
12 A Lambiotte reactor ; 128
13 Model of a vertical flow converter
charcoal plant. 141
14 A charcoal briquetting press. 225
15 Pillow-shaped charcoal briquettes . 225
16 A rotary kiln for activation of charcoal
in the Philippines. 232
Owing to the widespread use of cheap fossil fuels and
natural gas in industry, household charcoal has been somewhat
neglected during recent decades. The development of new
and improved charcoal techniques has nevertheless been
advancing during this period, unknown to outsiders.
Comprehensive charcoal literature has not appeared since
the late nineteen-forties; in particular, there have been no
publications concerned with industrial charcoal-making. Some
of the literature cited in this book exists only in
specialized collections. Occasionally the pUblic has learned
about the achievements of companies active in charcoal
production or equipment manufacturing, particularly in the
carbonization of biomass and the formulation of long-burning
charcoal fuels, but overall there has been an inadequate
flow of information to potential users .
The Commission of the European Communities,
Directorate-General for Science , Research and Development
intends to close the information gap by pUblishing this
handbook . However, a handbook cannot be expected to reach
all the innumerable small-scale charcoal-makers,
distributors and users, especially in developing countries,
who do not normally acquire knowledge of improved techniques
from books. At this level, information should be
disseminated directly by government agencies or where
appropriate, through internationally sponsored development
The author has been engaged as consultant and design
engineer in the charcoal and active carbon industry for more
than twenty years . He has also worked on assignments as
research and plant manager of charcoal and active carbon
plants . During these years he became aware, through numerous
contacts with Governments, Ministries of Planning and
private entities that two factors frequently prevent or
obstruct the promotion and realization of efficient projects:
inadequate knowledge of the state of the art
- xv -
lack of the experience needed to develop charcoal
The author's major concern in this handbook is to draw the
attention of all persons involved in energy project planning
to the fact that new and improved charcoal techniques are
able to convert forestal and agricultural wastes and
residues into energy. In countries which abound with these
reserves the modern charcoal-maker can make an important
contribution to the household fuel programme of his country.
For more than a thousand years, charcoal has been made
from whole trees; it is time for everyone to accept recent
advances in a very old industry and to adopt new ways. We
should always bear in mind:
THERE IS NO WASTE IN THE WORLD
WASTE IS AN ENERGY RESERVE
Therefore, let's use it.
The author would like to express his gratitude to the
numerous organizations which have contributed valuable data.
Among these are : the United Nations Industrial Development
Organization (UNIDO), the Food and Agriculture Organization
in Rome, and the Barbeque Industry Association i n the U.S.A.
Last but not least, the author would like to thank the
many charcoal producers and equipment suppliers who have
volunteered updated proprietary informat ion.
Neu-Isenburg, September 1984
- xvi -
HISTORY AND FUNDAMENTALS OF THE CHARCOAL PROCESS
1.1 Charcoal-Making from the Beginning until the Present Day
Prehistoric finds, dating back six thousand years, have
shown that arrow-heads were attached to their shafts by
employ ing wood tar, a material then obtainable only by the
charring of wood. Although we may never know when man first
made charcoal, extensive investigation has proved that in
Europe charcoal-making had already become an important
industry for the recovery of iron and other metals from
their ores around 1100 BC.
The Roman historian Plinius describes in his famous
Historia Naturalis (1) the method of embalming and preparing
bodies for burial in Egypt, in which the watery condensate
of the charring process was used as the preserving agent.
The more viscous parts of the condensates like tar and pitch
found applications as house paints, in the then flourishing
shipbuilding industry, and for caulking and sealing wooden
We may assume that charcoal was made mainly in open pits
at that time, but with very low yields. Later some
improvements were made by introducing the earthmound kiln,
which is still common in many developing countries today.
Although this technique is not at all satisfactory in so far
as the energy balance of the charcoal process is concerned,
it can be considered as an industrial step, because by
simple alterations one is able to collect some liquid
In 1635, the renowned chemist Rudol f Glauber (2)
discovered acetic acid as an essential component in the
condensate of the charcoal process . Immediately his
discovery drew the attention of the chemical industry to the
charcoal process as an available source of raw materials.
However, the earthmound kiln method did not permit the
production of the desired quantities of condensates (now
termed "pyrolysis oil"). Almost a hundred years were to pass
before the Swedish engineer Nordenschoeld (3) and the German
technician Reichenbach (4) designed commercial retorts by
which the energy balance of the process could be improved
considerably and the by-product yield was raised
sufficiently. The new "charcoal furnaces" spread throughout
most European countr ies and from there they were introduced
to the U.S. A. and Canada. The Swedish-German technology was
very successful and was only replaced by large-scale
equipment and improved techniques in 1850.
The growing demand for steel by industry in general, and
the enlarging capacities of the chemical industry, brought
about an unprecedented upsurge of charcoal and the liquid
by-products. Small and large-scale charcoal plants
mushroomed not only in Europe but also in North America. Not
only the number of production sites multiplied, but also the
capaci ty of the plants. This again emphasized the need for
better and more efficient technology.
Technical development was focused on continuous
processes and techniques to utilize the total accessible
energy contained in the raw material. Sophisticated
combustion systems were invented to generate heat or
electric power from the non-condensable gases of the process.
Despite these achievements (which resulted in better
charcoal quality), the steel industry and metallurgy
gradually turned to new resources for their blast furnaces :
refined bituminous coal, coke and lignite began to compete
with charcoal. The chemical industry also found that other
sources were more rewarding, namely bituminous coal and
later fossil oil and natural gas.
The already foreshadowed decline of the once-blossoming
charcoal industry became visible after the First World War .
Although a great number of plants had to be shut down, the
more advanced and well managed plants survived the crisis .
Then, with the economic recovery of the industrialized
countries, the demand for charcoal products revived.
Countries lacking in natural resources and therefore heavily
dependent on imports for all kinds of goods, curtailed their
spending of foreign currency and tried to exploit their own
reserves. Naturally, under these conditions, their forests
played an important role . Consequently the charcoal-makers
experienced a new peak within their exciting lifespan.
When the Second World War began, the charcoal industry
had in many countries a somewhat tactical task to sustain
the war machinery. The products provided by carbonization
plants were mani fold and far exceeded the expectations of
industrialists and businessmen a century ago.
Charcoal came to be utilized not only in metallurgy but
also in chemical processes and the fabrication of plastics,
it was the essential raw material for activated carbon with
its numerous outlets in the filter industry,
pharmaceuticals, catalysts, pollution control, etc .
Pyrolysis oil provided a basis for the production of organic
acids, methanol, aldehydes, acetone, creosostes, tars, etc.
In 1945, at the end of the war, the economy of many
European countries had come to a complete standstill. Again
the charcoal industry was hard hit. Survival meant
concentration and enlarged capacities, in other words
During the post-war years, a new technology was
commercially proved, the so-called "rapid pyrolysis", which
was first operated in the U.S.A. It had two major advantages
over previous processes : first, the carbon ization cycle
(residence time of the feed) was shortened dramatically,
thus making more profitable use of the invested capital;
secondly, the conversion of small raw material particles was
Rapid pyrolysis is one of the most important
achievements of charcoal technology. Whereas, until then,
the only feed for the charcoal plant consisted of pile wood
or wood logs cut to size, the new techniques permitted the
utilization of raw material up to a few millimetres in
diameter. This opened the door to a new category of raw
material resources until then untapped and neglected, namely
agricultural and industrial wastes and forestal residues .
One is tempted to say that these reserves, which abound in
developing countries, are almost unlimited . Their use to
provide household fuel, industrial charcoal and chemical raw
materials could make an important contribution to the
conservation of other natural resources, especially the
highly endangered forests.
When early man invented charcoal, its only use was as a
reductant to obtain metals from their ores. Numerous
applications have been added since then, and new markets
have opened their doors to the effective charcoal-maker.
Soon after the Second World War, people in industrialized
countr ies rediscovered the excellent properties of charcoal
for barbequeing. This specialized sector of the charcoal
industry has now become a major economic factor, comprising
also thousands of manufacturers of grills and utensils.
Sufficiently accurate data on the production and
consumption of charcoal and the by-products are difficult to
obtain. Besides charcoal, fuel wood is the main energy
carrier with which people cook their daily food in
developing countries. The world consumption of fuelwood, per
capita, including charcoal was estimated at 0.37 m3 in
1978 (5). However, in the developed world the per capita
usage reached only 0.13 m3, compared wi th 0.46 m3 in the
The United Nations Conference in Nairobi, 1981, (6)
concluded that approximately 2,000 million people are
utilizing firewood and charcoal for cooking and heating. For
several hundred million of them, it is already impossible to
find a sufficient supply of firewood because of the ruinous
exploitation of forests. Here the modern charcoal technology
with high-grade energy recovery systems can find a new task.
By tapping the vast waste reserves of the world, the
charcoal industry can make one of its most important
provide for the
in all developing
1.2 Theory of the Carbonization Process
Carbonization or dry distillation takes place when any
organic matter is raised to a high temperature (L, e. above
180 0 C) under strict exclusion of oxygen or under controlled
minimal air intake. Essentially the process of carbonization
follows a general temperature scheme :
between 1000 and 170 0 C all loosely bound water is
evaporated from the raw material.
between 1700 and 270 0 C gases develop (off-gas) ,
containing carbon monoxide (CO), carbon dioxide (C0 2),
and condensable vapours, which form pyrolysis oil after
scrubbing and chilling.
between 270 0 and 280 0 C an exothermic reaction starts,
which can be detected by the spontaneous generation of
heat and the rising temperature . At the same time, the
development of CO and CO 2 ceases but the quantity of
condensable vapours rises.
Once the carbonization process has entered the
exothermic phase , no more outside heating is required. The
temperature in the retort will climb slowly until it comes
to a standstill between 400 0 and 450 0 C.
Naturally, this scheme can be applied only if the
carbonization or dry distillation is conducted batch-wise.
To achieve a higher terminal temperature, the process must
be su~ported with extra heat from outside .
- 5 -
430000 l.-.-l -- 200
100 -::J ."
0 1 2 3 4 6 7 8 9
/ ~ , ,
'/ -~~ ,.
~ "'" - ~
- 20 ."
o lJ l.l __
5 --III 0 CIl -.... :.::: 50 --III 100 ."
o 1 2 3 456 7 8 9
Figure 1 Diagram of dry distillation (7)
Graphs-solid curve: temperature outside r etor t
doffed curve : temperature at retort centre
Bar diagrams-solid area : combustible gas
white area : C02
shaded area: condensate
2 3 4 5 6 7
__-+--+-t--t-+--1 100 ~
II -.... :.:::
Figure fa Temperature Diagram of dry distillation (7)
(After M. Klar , Techno/ogie d. Holzverkohlung)
- - - - 600 0 C
Figure 2 Temperature distribution
diagram (continuous process). (8 )
(From: W Emrich, Recycling in
Figures 1 and la are representative of the dry
distillation of European softwood and hardwood. They also
show the amount of pyrolysis oil which can be recovered
during the entire carbonization process.
During continuous carbonization the raw material moves
vertically, normally from top to bottom of the retort or
converter . The feed passes through various temperature
phases as stated above, one at a time (see Figure 2) .
Whereas the charcoal leaves the reaction container at the
bottom, the vapour-contain ing gases are drawn off at the top.
The mixture of gas and vapours expelled from a
continuous carbonization process remains uni form during the
desired period of time, e. g. for weeks or months. Another
advantage of continuous operation is its f lexibility in
relation to the residence time of the raw material and the
relatively short time it remains within the hot zone. Both
these characteristics have a great influence on the process
yield and the composition of pyrolysis oil or gas .
Many tests have shown that the pyrolysis oil containing
vapours undergo certain cracking processes on the hot walls
of retorts and tubes. These processes are enhanced by
prolonged residence times, thus undesired crusts and
depositions will occur.
1.3 Heating Systems for Charcoal Plants
To start up the carbonization and to maintain higher
temperatures, external heating is required. During the long
history of industrial charcoal-making, many heating systems
have been tried . All were intended to reduce expenses and
fuel costs. Only the three basic types shown in Figure 3
have survived and are in general use.
Off - gas
Off - gas
Internal heating by
of raw materials.
External heating by
combustion of firewood,
fuel oil or
Heating with recirc uıated
gas (retort or
converter gas). Hot
gases pass through
raw material charge.
F = Combustion chamber
Figure 3 Heating systems (9)
- 9 -
Charcoal pits a Concrete '"
Earthmound kiln brick kiln
METAL KILNS RETORTS/CONVERTER I 1 INTERNAL I I Portable I. Fixed HEATING SYSTEMS Vertical flow &: Fluid bed
Movable rotary disc
T---1 Mob ile
Brick re torts "
Metal Retorts Schwartz furnace
- _ T
HEATING GAS IN CONTACT
WITH RAW MATERIAL
Figure' Classification of charcoal processes
Tpye A: Most common system. Part of the raw material is
burnt under controlled air inlet. The combustion
heat provides the energy for maintenance of the
process. Recommendable only in loca tions Jhere raw
material prices are low (waste material).
Type B: Retort or converter heated from the outside under
strict exclusion of oxygen. Fuel can be provided
from the off-gases.
Type C: Very expensive heating system . Raw material comes
in direct contact with the hot gases. Charcoal and
by-product yields are high. Recommendable for very
large plant capacities only.
All the systems described are technically and
commercially proved. There will be advantages and
disadvantages which must be considered in making decisions .
Not only the costs for the investment will play a role, but
also the concept which the charcoal planner has in mind.
For the classification of charcoal equipment, the scheme
shown in Figure 4 is suggested for practical use. Presently,
more than one hundred concepts and methods to make charcoal
are known, all of which can be categorized and tabulated
within this frame.
1.4 Properties of Carbonization Products
Whether the charcoal or a charcoal derivative can be
regarded as a quality product will depend first on the
results of analytical tests . Chemical and physical
properties are greatly influenced by three factors - raw
material type, process characteristics, and after-treatment.
The latter refers to agglomeration and briquetting
techniques of the solid char, or to distillation and
fractionation methods applied to the pyrolysis oil and
residual process gas .
In any event, it is absolutely necessary during the
planning stage of a new charcoal venture to take a close
look at the applications and end-use markets of the expected
products (see Chapter 6). Specifications may be set by
individual consumers and can be obtained from them.
The terms and properties described below are intended to
acquaint the reader with the charcoal terminology. They
should be read carefully before proceeding to the following
1. 4.1 Charcoal
A precise and authoritative
becoming increasingly inportant
other imminent legislation.
definition of charcoal is
for label regulation and
Two typical published
1. Encyclopedia Sri tannica (0): "Charcoal is the residue
obtained when carbonaceous materials, of either animal
or vegetable origin, are partially burned or heated so
that tarry and volatile matter is removed; in most cases
the residues may be roughly described as impure carbon."
(Coal, coke and petroleum coke certainly are not
charcoal; but according to this definition they qualify).
2. Encyclopedia Americana (1): "Charcoal, a black, solid,
non-lustrous residue, or amorphous carbon, from
vegetable or animal sUbstances; or a coal made by
charring wood in a kiln or retort from which air is
excluded." (Dull bituminous coal is not charcoal but
according to this definition it qualifies.)
- 12 -
To resolve this dilemma we propose:
CHARCOAL IS THE RESIDUE OF SOLID NON-AGGLOMERATING
ORGANIC MATTER, OF VEGETABLE OR ANIMAL ORIGIN, THAT
RESULTS FROM CARBONIZATION BY HEAT IN THE ABSENCE OF AIR
AT A TEMPERATURE ABOVE 300 DEGREES CELSIUS.
This definition distinguishes charcoal from coke, which
is formed by carbonization of fluid organic matter such as
plastic coal or petroleum (when heated, coking coal becomes
plastic before it carbonizes) . It also distinguishes
bituminous coals and lignite from charcoal, because they
have not been subject to carbonizing temperatures during
The charcoal-maker differentiates between lump charcoal,
charcoal fines, charcoal dust, charcoal briquettes, pellets,
extrudates, and activated charcoal.
Yield: Expressed as weight of charcoal per unit weight of
dry raw material, in percentage. Note that the yield is
always applied to the dry material weight.
Specific Weight: Refers to the density of the charcoal,
which varies according to the density of the raw material.
The density of charcoal can be influenced within a narrow
range by the course of the process temperature, in
particular by the t e r mi na l temperature.
Hardness: A very important coefficient for industrial
charcoal. Standard scales have been imposed in some
countries; these are normally identical with the hardness
degrees of bituminous coal.
Moisture: After the charcoal has left the converter, it
vigorously absorbs water from the air up to 6 % of its dry
weight. In some continuous operations, the hot charcoal is
cooled by a controlled water spray. If treated in this way
or stored in the open, the moisture content may be much
higher than 5 to 6 %.
Content of Volatiles : If charcoal is heated to 900 0 under
confined conditions, it will lose weight because
hydrocarbons and nitrogen are driven out. This weight loss
is extremely important to industrial charcoal consumers when
def ining the utilization properties. In general, the weight
loss should not exceed 30 %.
Half-burnt charcoal, or "brands": Product with more than 30%
Red Coal: Same as half-burnt charcoal or "brands".
Fixed carbon content : The dry charcoal weight minus the
content of volatiles and i ncombus t i bl e s (ashes) is
equivalent to the content of fixed carbon, which also
determines its fuel value (Cf i x) .
Dead-burnt charcoal: This has a content of fixed carbon
which results in difficult ignition of the charcoal.
Ash content : The ash is composed of the natural minerals
contained in almost any organic matter and contaminations.
The quantity is related to the composition of the raw
material mix, e. g. wood branches with a high proportion of
bark will give high ash containing charcoal. Charcoal ashes
are distinguished by their solubility in water and by
Sulphur and phosphorus content : The low sum of these
substances normally found in charcoals make them especially
attractive for use in blast iron furnaces and for
metallurgical purposes . The desired value for sulphur is
usually below 0.05 % and for phosphorus under 0.03 %.
- 14 -
Heating or calorific value: This depends on the fixed carbon
content and will be lowered only by high ash content. In
general, heating values range between 6,500 and 7,200
kcal/kg (30,100 KJ/kg), comparable to bituminous coal.
Active surface: The surface of well burnt charcoal is
porous. The porosity makes charcoal easy to ignite, reactive
in chemical processes, and able to absorb substances and
remove them from liquids or gases. The porosity can be
measured, and is expressed in m2/g.
Active or activated charcoal: The porosity or surface area
can be enlarged by special activation processes. Industries
use gas, steam or chemical activation. The largest surface
area which can be achieved in commercial plants measures
approximately 1,500 m2/g, which is close to the area of a
Agglomerated and briguetted charcoal: Some
applications and major barbeque markets demand
with a particular shape. Known shapes and forms
cylinders, hexagonals, diamonds, bricks,
pillow-shaped conglomerates and pellets. The
parts are: charcoal, binder, additives .
Energy extender, cooking-time extender: These are inorganic
substances which are added to barbeque briquettes to prolong
cooking time. They slow down combustion time and retard the
heat release of the fuel .
Gas generator or producer gas
engines for the generation
alternative fuel for gas-fired
1.4.2 Pyrolysis Oil
The oil varies very much with the type of raw material.
It contains more than one hundred different substances,
which once made it a valuable feedstock for the chemical
industry. Its growing importance for developing countries
stems from the fact that it is a feasible substitute for
industrial fuel oil.
Viscosi ty: This can be controlled by the addition of water,
and is measured according to normal standards.
Acidity: Measurement is by analytical titration, without
relating the acidity value to particular acids.
Organic fatty acids: These are
pyrolysis oil. The most important
butyric acid and propionic acid.
regular constituents of
acids are acetic acid,
Pyrolytic alcohols: Mainly methanol as a regular ingredient
of pyrolysis oil.
Calorific value: This is related to the raw materials.
Conifers yield oils with high heating values.
Flash point: Determines the ignition properties and is an
essential criterion for all boiler fuels.
Flame tempera ture: Measured under stoichiometric condi tions
(in an environment of balanced oxygen).
Corrosivity: Pyrolysis oil is aggressive to mild steel.
Stainless steel, copper, ceramics, plastics and wood are
Ashes: These are incombus tible particles
into the pyrolysis oil. Reasons:
equipment, contamination during storage.
which have entered
Solidifying point: The temperature at which the residues of
pyrolysis oil lose their flow characteristics.
Pour point: The temperature at which the residues of
pyrolysis oil start flowing.
1.4.3 Process Gas
This is the gas which leaves the retort or converter; it
is therefore frequently called retort or converter gas.
A distinction is made between two types of off-gas which
have different commercial values:
(a) Off-gas that is not passed through a scrubber/chiller
system. It contains the pyrolysis oil vapours and is usually
referred to as "high Btu converter gas", meaning that it has
a high calorific value.
(b) The residual gas which has passed through a
scrubber/chiller system and has been stripped of the
pyrolysis oil vapours. It is frequently referred to as "low
Btu converter gas", meaning that it is a heating gas of poor
calorific value. It is composed of CO, CO2 hydrocarbons,
nitrogen and water vapour.
(1) Plinius, Historia Naturalis, Lib. 11, de pice (23 - 79)
(2) Glauber (1604 - 1670), Miraculum Mundi, 1653
(3) C.F. Nordenschoeld, Abhandlungen der Koeniglichen
Schwedischen Akademie der Wissenschaften, Jahrgang 1766
(4) Karl Freiherr von Reichenbach (1788 - 1869)
(5) FAD Forestry paper No. 41, Rome 1983
(6) U.N. Conference on New and Renewable Sources of Energy
Preparatory Committee, 1981. Report of the Technical
Panel on Fuel Wood and Charcoal on its Second Session.
(7) M. Klar, Technologie der Holzverkohlung, 1910
(8) W. Emrich, Recycling in Developing Countries, 1982
' (2 10 - 214)
(9) CARBON INTERNATIONAL, LTO., Neu-Isenburg, FRG, company
(10) Encyclopedia Britannica, Vol. 5, 1951
(11) Encyclopedia Americana, International Edition, 1964.
TRADITIONAL METHODS OF THE SMALLHOLDER CHARCOAL-MAKER
Traditional carcoal-making, which has a long history, is
characterized by the following main features:
Zero or low investment cost ;
Use of construction materials which are at hand on the
site or available nearby, e.g. clay, soft-burnt bricks;
Zero or low maintenance costs achieved by avoiding metal
parts in the kiln construction as far as possible;
Manpower is not a major concern;
The normal raw material consists essentially of wood
logs and coconut shells; other types of biomass may be
By-product recovery is limited owing to the fact that no
sophisticated equipment is employed;
It is typically a family or cooperative business.
Much of the charcoal in the world has been made by families
or small businesses run on the above lines, using simple
technology and low capital investment. Although the
technology is simple, it is nevertheless precise and
skilful, as will be seen in the following sections. Modern
industrial processes are discussed separately in Chapter 3.
- 19 -
2.1 Charcoal Pits and Earthmound Kilns
To save transportation costs, the small-scale
charcoal-maker produces his char at the place where he
collects the raw material. Because of his frequent movements
from site to site, he cannot employ heavy equipment.
Both the pit method and the earthmound kiln offer
appropriate solutions. Both require skill, patience and
readiness to observe correct working methods at all times
and in all weathers. Therefore, the business of
charcoal-making with all its "secrets" is usually handed
down from father to son and is well guarded by the family.
An important part of charcoal-making experience concerns
the insulation of the charcoal pit or earthmound and the
control of air flow. If not properly controlled, excess air
will cause the charcoal to burn away to ashes and destroy
the result of several days' work in a few hours.
The use of earth to keep out oxygen and to insulate the
carbonizing wood against excessive heat loss surely goes
back to the dawn of history. It is, therfore, worth-while to
study its advantages and disadvantages. Obviously this
method has survived because of its low cost. Wherever trees
grow, earth must be available and mankind naturally turned
to this cheap, readily available non-combustible material as
a sealant to enclose the carbonizing wood .
There are two different ways to use an earth barrier in
the charring process : one is to dig out a pit, put in
firewood and cover the whole with excavated earth to seal
and insulate the chamber. The other is to cover a pile of
wood on the ground with earth, sand and leaves. This cover
forms the necessary gas-tight layer behind which charcoaling
can take place. Both techniques, if properly carried out,
can produce good charcoal within certain limitations. But
these methods are wasteful of resources.
The pit and the earthmound methods have been studied by
many researchers in the last century (1). According to their
results the fixed carbon content (Cf.) of the IX
varies between 65 % and
15 % based on the weight
charcoal produced in those kilns
80 %, the yields rarely exceeding
of the dry fuelwood charge.
Statements that the recovery rate of a charcoal pit or
an earthmound operation is "well over 20 %" must be regarded
as unfounded. Because of the fact that a significant
depletion of wood resources allover the world can be
observed as a consequence of wasteful charcoal conversion
and the rigid arguing of their defenders, it seems quite
appropriate to shed some light on the complexity of the
Charcoal conversion efficiency can be defined in terms of
charcoal output (kg)
wood input (kg)
charcoal output (MJ)
wood input (MJ) .
While ~ can easily be calculated if the energy
content of wood and its char yield is known, the
weight-based efficiency criterion ~w varies depending on
just how one defines charcoal. Unfortunately, there is no
universally accepted def inition of charcoal. However, most
of the literature on carbonization agrees that - measured on
a dry weight basis - charcoal should exhibit a fixed carbon
content of at least 75 % (the other principal components are
hydrogen: 4.1 %j oxygen: 15.2 %j nitrogen: 0.8 %j and
minerals: 3.4 %).
On the input side, the biomass source wood is composed
of cellulose, lignin, hemicellulose, extractives and
minerals. In terms of chemical composi tion, one can
distinguish between hardwood and softwood: on the average,
hardwood contains about 43 % cellulose, 23 % lignin and
- 21 -
35 % hemicellulose, whereas softwood usually contains 43 %
cellulose, 29 % lignin and 28 % hemicellulose. These
di fferences in composition affect heat content i the higher
the lignin and extractives content, the higher is the gross
calorific value of wood.
In the process of pyrolysis, lignin promotes char
formation and holocellulose (cellulose and hemicellulose)
promotes the 'release of volatiles . The heating value of the
primary end prodct - i. e. the charcoal - is determined by
its carbon content. The general equation describing the
relationship between carbon content (C) and higher heating
value (HHV, dry basis) of combustible fuels can be
approximated by the following equation (2).
HHV = 0.437 x C - 0.306 (MJ/kg)
wich is illustrated in Figure 5.
Another relevant factor here is the species- and
age-dependent moisture content of wood, which directly
a ffects the net heating value, the ignition properties and
the efficiency of fuel utilization. Fresh wood may have a
moisture content of as high as 67 %, which is also the
practical limit of combustibility. On the average, hardwood
contains 30 .2 % moisture, and softwood about 46 %. The
following formula (Tillmann, 1982) can be used to calculate
the net heating value of wood as a function of its moisture
NHV (MJ/kg) = HHV - 0.2 33 x MC
NHV = net heating value (MJ/kg)
HHV higher heating value (MJ/kg)
MC = moisture content.
Carbon Content and
Higher Heating Value
Moisture Content and
Net Heating Value of
Average Tropical Wood
L..----f--+--+--+--+---1f----+--+--+--+-...... MC (%)
10 20 30 1,0 50 60 70
Assuming that the higher heating value of average
tropical (dry) wood is 20 MJ/kg (3), the curve presented in
Figure 5a can be derived from the above formula.
Thus, if the Cf i x of dry charcoal is defined as 75 %
(which is equivalent to approx. 30 MJ/kg), and if the
chemical composition of the wood biomass as well as the
characteristics of the conversion technology are known,
7, w or 't e can be regarded as a function of the moisture
content of the wood. The relationship between efficiency and
moisture content can be expressed as a curve which has the
same shape as the curve in Figure 5a; however, for a given
biomass input, the precise position of the efficiency curve
is a function of the carbonization technology employed.
2.1.1 The Charcoal Pit
Virtually, there are numerous ways to build a charcoal
pit and all need very little skill.
The basic principle is to lead the air from one end of
the chamber to the other flowing on the bottom. Therefore,
before charging the charcoal pit with the fuel wood bedlogs
are laid forming some kind of a crib on which the charge
will be placed.
The crib is made from logs, cut to the width of the pit,
and they are laid evenly spaced along the entire length.
On top of this first layer a number of logs will be
placed each equal to the length of the charcoal pit.
Later when the charge has been lighted the incoming air,
mixed with the hot gases, will travel beneath the charge and
heat it up to carbonization temperature, until they leave
the chamber through the flue on the opposite side.
After loading the pit is covered with a layer of leaves
normally 20 cm thick and on top with a layer of soil of the
- 24 -
In a typical pit operation burning takes place progressively
from one end to the other.
The produced charcoal of larger pits is not very
uni form, because the burn is di ff icul t to control. Smaller
pits are more efficient, because they have a better airflow
The large charcoal pi t normally takes 25 to 30 m3 of
fuel wood per burn and the wood is cut in length of 2,40 m.
Miniature pits with a capacity of 4 to 5 m3 are frequently
in use. Their conversion efficiency is very poor and the
charcoal produced of inferior quality. In Figure 6 the
cross-section of a larger charcoal pit is shown with the
Because it is very difficult to control the airflow in a
pit and the internal temperatures a lot of the fuelwood
charge is burnt to ashes. Another portion remains only half
burnt. Because of false circulation of the gases it was
never dried out and properly heated.
A further problem is connected with falling rain. The
pyroligneous gases tend to condense in the foliage layer and
in the earth used as outer cover. Therefore when rain falls
those condensates are washed back and down to be reabsorbed
by the charcoal (5). They will cause later damage to
jutebags by rotting them and the charcoal when used in
housholds releases unpleasant smoke.
Pit sites should be selected where a deep stratum of
soil can be expected. Where the soil is loose the vents of
the pit must be timbered.
In many cases and for large pits steel sheets are used
for cover before the soil is put on top, thus preventing
contamination of the charcoal by falling soil when the kiln
is uncovered at the end of the carbonization.
According to the FAO Forestry paper No. 41 (4) a team of
five men can produce from a pit size of 6 m x 2.70 m x
1.20 m (depth at the igniting point) and 2.40 m depth at
opposite side 360 tons of charcoal per year .
This would have resulted in USD 70.00 per ton in 1983 .
The indicated cost is for charcoal at the kiln site ready
for transportation. The calculation, however, does not allow
for labour overhead and profits.
2.1.2 The Earthmound Kiln
The typical smallholder charcoal maker builds a kiln of
about 2m in diameter at the base and approximately 1. 5 m
high as shown in Figure 7. Approximately six to ten air
inlets are installed at the base. The smoke and the gases
developing during the carbonization are drawn-off at the top
through an opening of 20 cm in diameter.
This describes roughly a round earthmound kiln. However,
one can find other shaped kilns like rectangular mounds in
use as well .
For the preparation of the kiln si te sufficient space
has to be cleared, levelled and if necessary compacted also.
In the case of rectangular or square shaped mounds it
becomes necessary to erect posts, several on each side,
which give stability to the wood pile and provide a support
for the operator when he is covering the kiln with leaves,
soil or metal sheets.
Again, as with the charcoal pit, it is most important to
provide a good air and gas flow within the mound after
lighting. This will be achieved by forming a grid of crossed
small logs (maximum diameter 10 cm) which are first laid out
and arranged on the ground. On this platform the fuelwood
will be stacked.
For the stacking of the wood exist no strict rules and
the piles are set up very differently. In general one can
say that in spheric earthmound kilns the charcoal maker
arranges it vertically and in other mounds horizontally.
- 27 -
-J wOl '0
- 28 -
All gaps between the logs or branches are filled in with
smaller woodlogs, off-cuts, etc. to make the pile as compact
as possible which facilitates the direct heat transfer when
the carbonization has started.
Also special care has to be taken to the surface of the
pile that it shows an even profile and makes a good support
for the cover of leaves and soil.
The lower layer of the cover is made with leaves, straw
or grass. On top a sandy soil or loam are applied
approximately 20 to 25 cm thick.
An important improvement can be achieved by putting in
metal sheets before the outer soil cover is made. This will
reduce defilement of the charcoal by dropping of soil down
duri ng the carbonization, when the mound is slowly sinking,
and when it is uncovered at the end.
These metal sheets can be gathered from scrap or cut out
of spent oil drums. Depending on the usage they will,
however, corrode in a more or less short time and have to be
replaced then. Recent calculations have shown t hat this type
of operation may become quite costly in countries where
scrap prices are high.
The igniting of a kiln is ' done either through the air
inlet holes on the base or through the centre hole at the
top. In every case, to enhance the firing kindling wood, oil
soaked fabrics are used or a shovelful of glowing charcoal
is put into the centre hole on the kiln top.
After the kiln has "caught fire" the operator observes
carefully the colour of the smoke exi ting the mound. Dense
white smoke will be issued for the first day or days
indicating that the water of the fuelwood is being
After this initial period, the length of the time
depends on the size of the kiln, moisture content of the
charge, thickness of the woodlogs, etc., the smoke will turn
blue and becomes clear eventually.
PHOTO I Small Earthmound kiln in Ghana one hour
after lighting. (Photo W. Emrich)
PHOTO 2 Discharging charcoal from same kiln
two days later. (Photo W. Emrich)
"tJ w5 0
E 01 .S
III .... III U .'..-. CI> CI> c:: '- ~ CI> U
CI> -'-. '..c:: c::
<:) - E-..e..
The skilled operator feels frequently the walls of the
kiln for cold or hot spots and uses a wooden stick for
probing the conditions of the wood charge and searching for
Based on his findings he closes or opens the vents at
the kiln base.
Besides these observations he must look for cracks in
the kiln cover which do appear during the entire
carbonisation cycle, due to the continuous shrinking of the
charge and in the same grade as charcoal is formed. Cracks
must be sealed immediately to prevent the influx of air
which would cause burning of the fuelwood to ashes.
When charring is jUdged complete, all vents and the
centre hole at the top will be closed and sealed with earth.
For the sealing of larger kilns clay and stones are used.
The cooling time of the kiln depends also very much on
its capacity or size . It may take a few days or up to
During the cooling phase the kiln remains under
permanent supervision, and must be kept airtight. Otherwise
the charcoal inside catches fire and starts glowing which
prolongs the cooling time considerably.
When the earthmound kiln has cooled out it is uncovered
and the charcoal crop separated from fines and "brands" by
screening or other simple means and made ready for sale .
Photo 1 and 2 show the beginning and the end of an
earthmound charring cycle of a small kiln, as usually
carried out. They also reveal that the operator does not
display great skill. Obviously the obtained charcoal crop is
of poor quality and defiled with soil.
Earthmound kilns can be enlarged up to a diameter of
15 m and over, whi th space capacities of 150 m3. However,
large scale earthmound kilns have to be modified and their
construction needs very much skill.
- 32 -
They require centre firing canals as shown in Figure 7.
Some details of such a canal structure can be seen in
Figure 8. also, which refers to a special kiln type
described in the following section.
2.1.3 The Earthmound Kiln with Chimney
These modified kilns represent the most advanced group
of the earthmound family. They have been developed in Europe
during the middle of the last century, namely in Sweden and
in the western parts of Russia.
Very large amounts of charcoal had been produced with
these kilns for the growing iron smelting industry.
The elements used for the kiln construction are
basically the same as described in the previous section; the
grate formed with woodlogs on the bottom, the fuelwood pile
(stacked vertically) and the centre hole for firing.
However, in addition a chimney is attached (normally only
one) which is connected to the pile by an underground flue
The significant improvements rest with this chimney.
Since the diameter of it can be determined according to the
oxygen demand the kiln can be precisely controlled with the
draft of the chimney, which depends also on the height of
it, resulting in a higher yield of better charcoal.
Whereas, the traditional earthmound kiln takes the air
in through numerous inlets with undefined cross-sections,
which will change during the carbonization cycle also (due
to the shrinking movement of the kiln shell), the chimney
secures an uniform air influx throughout the whole operation
The investment costs of these kilns are naturally higher
and, therefore, normally metal scrap is used for the chimney
construction. Frequently oil drums are welded together and
make a good chimney. However, one has to bear in mind tha t
- 33 -
pi 11 ar
Chimney made of oil drums
Centre fire hole
Figure 9. An earthmound kiln with chimney.
the opening of the smoke stack may have to be reduced and
adapted to the size of the wood pile.
In many cases a stack made from firebricks is employed
thus eliminating corrosion problems. These chimneys are
preferred in charcoal operations with large plant sites and
where the fuelwood is permanently carried to.
Figure 9 shows a medium size earthmound kiln with an
attached chimney assembled from spent oil drums. The centre
pillar as shown in Figure 9 guarantees the firing of the
wood pile from top to bottom at the same time. The
carbonization will progress from the centre to the edges
almost equally and within the entire height of the kiln.
Chimney kilns are usually lighted with a torch. During the
operation the same observations and probings are necessary
as already mentioned in the section dealing with regular
Owing to the higher temperatures which can be achieved
the charcoal produced in these kilns has a low content of
volatile matter and consequently a higher heating value as
compared to normal earthmound charcoal.
One disadvantage which is connected with all kilns
having a loose shell has to be seen in the always present
danger of showing cracks during the carbonization and
This contributed to the fact that many charcoal
producers turned to kilns with fixed shells, which are
represented by the hangar and round grill types and which
will be described later.
2 .1.4 The Earthmound Kiln with Tar Recovery
It is only a small step from the chimney-kiln to the
charcoal operation with tar recovery. A few but important
modifications within in the chimney section are necessary.
- 35 -
::J "tl !!
lll ..... ~
- 36 -
In the first circumstance the chimney is designed to
expel all gases generated during the carbonization process
into the ambient atmosphere. In the latter case the chimney
serves two purposes: condensing part of the gases and
guiding the uncondensable portions to the outside.
Since the investment cost would not allow the
installation of chiller and scrubber systems the earthmound
operator has to limit himself to the collection of only part
of the charcoal by-products. In this case it will be mainly
From 100 steres of wood normally 25 tons of condensate
can be recovered (8) . It consists of water, acids and tar .
In practice about 2 tons of tar can be recovered from it (9).
Since all wood tars contain a high proportion of heavy
organic chemicals with higher melting and boiling points the
condensation of them by aircoolers is quite efficient.
For this reason, the way the hot gases travel through
the stack, has to be extended to allow them to dispose of
part of their tangible heat within the chimney area,
resulting in partial condensation.
This can be accomplished by putting in the chimney some
metal sheets which force the gases to flow around them and
do not permit them to escape on a direct way.
Figure 10 displays the simple design for a three
sectional kiln stack made from oil drums.
In many cases a higher chimney will be required to
provide an adequate travel route for the gases.
The condensed tar and oils will be collected at the
bottom of the stack and lead through a pipe into the storage
The structure of the wood pile with supporting grate
beneath and the shell are built in the same manner as with
Of course, some special structures have been in use with
more or less significant effects. The best results the
author has achieved were with fixed shell kilns of the
hangar type and with a modified Brazilian Beehive kiln.
The economics which can be achieved by the recovery 0 f
charcoal by-products will depend very much on the use-market
prices for them. In 1983, according to a market survey
performed by the author in African and some Asian markets
the production cost for charcoal in earthmound kilns ranged
between USD 48.00 and 62.00 per ton of lump charcoal. Tar
sales would have reduced the production cost by USD 15.00 to
22.00 per ton.
2.2 Charcoal-Making with Portable and Movable Kilns
These kilns are made by modi fying oil drums or other
containers or are specially designed and built from metal
sheets. The latter consist of few sections. They are rapidly
assembled or dismantled by the charcoal burner, using simple
Kilns of this kind have been made since the beginning of
the century (the Delhemmeau Kiln, 1907) (7), as an easier
means than the traditional stack, for the production of
charcoal from bulky sawmill waste and the branches and
brushwood left after felling. Interest in them quickened
when it was found practically and economically feasible to
use charcoal gas-producers for propelling motor vehicles.
But the use of these kilns reached its maximum in some
Western European countries during the 1939 - 45 war when
petrol supplies were short and charcoal became by far the
most commonly used fuel for combustion engines. The vogue of
portable kilns passed with the return of normal fuel
supplies to these countries. The kilns are now made by only
a few of the many manufacturers of ten years ago .
In this type of kiln, carbonization is discontinuous,
being carried out by the combustion of part of the timber to
be carbonized. For the most part, these kilns work on the
downward, rarely direct, draught principle. Observations
(10) made with the help of regularly spaced pyrometers
ins ide ki lns of the stack type show that carbonization works
in the same direction as in the traditional pit or
earthmound kiln, e. g. from the top downwards and from the
middle outwards. Carbonization temperature is usually 440°C,
but may be higher and even slightly exceed 600° C during
Portable kilns have one great advantage over the
traditional stacks in that they appreciably reduce the time
of the carbonization operation (about 48 hours), chiefly
because the preliminary "dressing" of the stacks with earth
is dispensed with. Moreover, the carbonization process
requires much less surveillance, so that there is some
economy in manpower. Furthermore, the charcoal produced is
free from earth and gravel and this is important where it is
to be used for gas-producers or combustion engines.
The chief criticism directed at these kilns emphasizes
that they do not facilitate the collection of by-products,
and that their charcoal yield is low compared with the
weight of wood carbonized (4). The yield, however, can be
appreciably increased if the various operations are carried
out carefully, especially charging and control of the air
2.2.1 The Tongan Oil Drum Kiln
The Tongan oil drum kiln is a low-capi tal, small-scale
method of producing charcoal from wood (11).
As the name suggests, this kiln was developed in Tonga
when the need arose for a low-cost method for converting
coconut shells and wood to a salable product . The solution
was a simple-to-contruct and use charcoal kiln made from a
200 litre drum. Other drum kilns have been made in the past,
but because of their design have not been particularly
efficient or easy to use. The Tongan kiln, however, takes
advantage of the drum shape to produce good quality charcoal
The key to the Tongan design is the opening, about 20 cm
wide, which is cut along the vertical side of the drum (see
Figure 11). With the drum lying on its side and the opening
facing the prevailing breeze, a fire is built inside. The
drum is rolled so that the opening reaches a progressively
higher position. This allows more and more firewood to be
added until the drum is completely full. It is important
that a good fire is kept burning without being smothered by
the addition of new wood. As the fire burns down, more wood
is added - the whole process taking up to an hour. When no
more wood can be added and the fire is burning strongly, the
drum is ready to be sealed. (The charring process has
already begun in the lower part of the drum where the air
cannot reach). The drum is rolled over so that the opening
is facing the ground. Clay or sand is packed around the
bottom so that no smoke can escape. At this time, the entire
drum is sealed and can be left for 6-8 hours to cool. When
it is completely cool, the drum can be rolled over again
and the charcoal removed (see Figure 11).
The Tongan kiln possesses several advantages:
Low cost: The only costs involved are the drum and the
tools to cut it open (hammer, chisel, bush knife).
Transportable: One person can carry it to the si te of
Simple to use : There is less danger of being burned
than with some larger kilns and retorts because the
major movement is by rolling and the small size makes
the fire manageable. It does not require highly skilled
per kilogram of
have shown that the output of charcoal
firewood equals that of the larger
It can deal with small amounts
merely to increase the number
quantities are to be processed.
The disadvantages are:
of firewood. One needs
of drums if greater
Firewood must be cut to fit the drum.
Drums last at most 6 months.
Charcoal in contact with the ground during the
part of the process may absorb moisture. To
this, the original section of the drum that was
to make the opening can be replaced as a door
2.2.2 The Philippines Kiln
This kiln was first designed and used in the
Philippines, in particular for the carbonization of coconut
shells . It employs an oil drum set up vertically (12) .
The Philippines kiln is made from an old oil drum in
which the top and bottom lids are still firmly in place.
Reject oil drums can usually be bought cheaply at oil
company depots, and these are quite suitable. In addition to
the drum, a flat circular sheet of thin metal, about
50-54 cm in diameter, with a central hole 10 cm in diameter,
is required. This forms a movable lid for the kiln. For
convenience, a handle can be bolted or tack-welded onto this
lid. A smaller piece of flat metal 15 cm in diameter is used
to form a cap for the central hole in the lid when
charcoaling is completed.
The kiln is constructed as follows. At the top of the
drum there are two holes. The plugs should be removed from
these holes and, using an oxy-acetylene welding torch, the
- 42 -
Top of drum
( becotnes bottom)
4 holtls (S em dia.)
for kiln air inlet
Cover for hole in lid
Lid (50 em dia.) with
10em hot« and handlt'J
Hole (45 em dia.) cut in
top of lid leaving rim
Figure 12 The Philippines oil drum kiln
- 43 -
smaller one is cut out so that it is as big as the larger
one (see Figure 12). Two more holes are cut in the top of
the drum, the same size as the larger hole and positioned at
the same distance from the edge of the drum and midway
between the first two. At the opposite end of the drum, a
circle of metal about 48 cm (16 inches) across is cut out.
The drum is now ready for use, the end with the four holes
forming the bottom of the kiln (see Figure 12).
To operate the kiln, it must be positioned securely on
bricks or pieces of metal pipe or rail about 5 cm high, so
that the air holes are not blocked. Alternatively, a round
hole about 50 cm in diameter can be dug in the earth over
which the drum is placed. Air channels must be dug under the
edge of the drum so that air can freely enter the air holes.
After the drum has been filled with coconut shells,
leaving a hole about 15 cm across by 15 cm deep at the top,
paper, coconut fronds, or an oily rag are placed in this
hole and the fire is lit at the top of the kiln. When the
f ire has "caught on" (this will take about 5 minutes), the
lid is placed on top of the kiln. Dense whi te smoke should
issue from the hole in the lid.
If flames are seen, there is too much air entering the
kiln. The small centre hole in the lid must be covered with
a flat piece of metal, so that only white smoke continues to
emerge. The air entering the bottom of the kiln through the
four holes should be controlled by banking up earth or sand
around the bottom of the kiln so that only two small gaps
(5 cm by 1 cm) on opposite sides of the kiln remain.
As the shells are converted to charcoal, they reduce in
volume. The lid should be removed and the kiln refilled with
shells about three times at 3D-minute intervals. After about
2 1/2 hours, the smoke will decrease in quantity and change
from dense white to pale blue-grey. When the kiln has
virtually stopped smoking, the cap should be put over the
top hole, and the cap, the kiln lid and the bottom of the
kiln must be sealed securely with sand or earth so that no
- 44 -
air can enter the kiln. Any air entering the kiln will
reduce the charcoal yield.
Four hours after sealing, the kiln should be cool to the
touch and ready for discharge. Each kiln should yield
12-25 kg of charcoal per firing. A single worker should be
able to operate up to 10 kilns on a daily cycle.
2.2.3 The Black Rock Forest Kiln
This kiln is in one piece, the part being electrically
welded to form a bell of steel sheeting. The dimensions are
shown in Figure 13 . Capacity is about 2.8 m3
The lower part is pierced with holes, 4 for the
reception of steel smoke outlets, the others acting as air
intakes. The upper part has a hole fitted with a metal cap.
The kiln was designed with a view to its use as part of
a fixed charcoal burning yard, consisting of four kilns
which can be hoisted on to eight cement emplacements . The
latter are distributed in a circle, in the centre of which
is a derrick for moving the kilns (see Figure 14, 15).
Large stocks of wood are piled near the emplacements,
and while carbonization is taking place on emplacement A,
with kiln no. 1, (Figure 15), the crew prepares the stack on
emplacement B. When carbonization is completed on
emplacement A, number one kiln is lifted therefrom and
placed over the stack already prepared on emplacement B.
Firing takes place at once, and while carbonization is in
progress the crew sacks the charcoal made on emplacement A
and prepares the fresh stack on A.
When carbonization is completed
on empl acement B,
stacked wood on A,
process is repeated
0, E, F, G, H, and
no slack periods in
kiln is hoisted and placed over the
so on. It can be seen that when this
each of the emplacements A, B, C,
each of the four kilns, there are
crew's working time.
2 = Lid for ignition hole
3 =Air inlets at the bottom ,= Chimney
5 =Hoisting rings
Figure 13 The Black Rock Forest kiln .
Figure 14 Handling the kiln with a derrick.
®:: 4 ARM OF F0 DERRICK 0 0
A - H = Concrete emplacements for kilns
1 - 4 = Kilns in operation
Figure 15 A battery of four Black Rock Forest
kilns in operation
Preparation of the wood. Logs are laid radially on the
emplacement, leav ing channels between them to correspond to
the air intake holes in the base of the kiln. The wood grate
is laid on the logs and the wood is arranged in
stack-formation on it. The shape and position of the central
chimney are fixed by a vertical steel cylinder which fits
into a cavity in the emplacement. Immediately around this
pipe, dry brush-wood is heaped and the wood to be carbonized
is heaped to the top of the kiln. The steel cylinder serving
as a guide for the central chimney is removed afterwards.
Lighting. When the wood has been stacked, it is covered
by the kiln which rests directly upon the cement
emplacement. Earth is piled all around the edges of the kiln
to prevent the passage of air.
The kiln can be lit either by means of the central
chimney, introducing embers and dry brushwood through the
central hole, or by thrusting embers through a tube inserted
into one of the base inlets. In the latter case, the central
chimney is filled with brushwood during the stacking
When the fire is well alight, the upper hole is blocked,
the smoke-outlet pipes are inserted, and carbonization goes
on until flames appear at the lower holes. These are then
stopped up in turn and the stack is allowed to cool.
2.2 .4 Sectional Metal Kilns
of these kiln types have been on the
Especially during war times the army
to obtain a clean charcoal for their
markets and in use.
employed these kilns
They all consist of at least one cylindrical section
with a conical cover and two or more smoke stacks. an the
kiln base are usually four air channels fitted and the cover
is provided with four equally spaced steam release ports.
- 48 -
The kilns are made from sheet metal and can be built by
local craftsmen in a workshop which has basic welding,
rolling, drilling and cutting equipment.
Figures 16 and 17 show a sectional kiln and the way the
wood grate on the bottom of the kiln is arranged.
The principles which apply for the charging and
operation of the earthmound kilns described in the previous
sections are almost the same for the sectional metal kilns.
The popularity and the widespread use these kilns once
enjoyed is mainly due to the fact that their sections can be
separated and carried to another plant site.
However, several facts have hampered their promotion
made the kiln
during the past five to ten years gradually:
rising iron and steel prices have
unaffordable for many charcoal makers
the kiln shell, if not
can be deformed during
machinery which would
the kiln tends to corrode and the lifespan is short in
comparison with firebrick kilns.
properly designed and contructed,
operation and the repair requires
be rarely available in a remote
The Tropical Products Institute (TPI), a scientific unit
of the Overseas Development Organisation of the U.K. has
gained considerable experience in operating sectional metal
kilns of various design. The institute has evolved a kiln
with good durability which is considered to be optimal in
The institute recommends a two sectional kiln,
consisting of two interlocking cylinders with a conical
cover. The kiln is supported on eight air inlet/outlet
channels, arranged radially around the base (13).
During charring four smoke stacks are fitted onto
alternate air channels. The cover has four equally spaced
steam release ports which may be closed off with plugs.
- 49 -
rfJ 0,10 m gJ 0,45 m
Figure 16 A portable metal kiln
Figure 17 Air inlet channels at the
boHom of a portable metal
kiln with wood grate
The size of the wood to be charged to the kiln must not
exceed 60 cm in length and the maximum diameter is 20 cm.
Wood with a diameter greater than this should be split
before kilning. The TPI kiln takes approximately 7 m3 of
After placing the lower section of the kiln onto the
supporting air inlet channels the bottom of the kiln is laid
out with stringers forming a grate. Care has to be taken,
that the air channels protruding into the kiln are not
blocked by the wood charge.
The fuel wood is normally placed horizontally in
successive layers, filling in as many gaps as possible. It
is advisable to place the thicker logs in the centre of the
kiln where they will be more exposed to the heat as close to
For the lighting of the kiln several points at the base
will be prepared with kindling material and for the ignition
a flame is necessary.
During the carbonization colour of the smoke, wall
temperature and leaks have to be watched. For the cooling of
the kiln all openings are closed and the smoke stacks were
taken down before.
The author has experimented with various kilns of the
TPI type in East Africa and has established the following
working schedule with hardwood (acacia d.):
Two experienced operators
lighting and draft
Charr ing time
- 51 -
08:00 - 10:00
10:00 - 13:00
08:00 - 10:00
For the operation the following tools were in use:
one crosscut saw, one axe, two wedges, one sledge hammer,
one cutlass, one rake.
According to the TPI the following materials and their
quantities are necessary for the construction of the kiln:
Top and bottom
Bottom r ing
SO mm x SO mm x
3 mm mild steel
3 mm m.s. sheet
3 mm m.s. sheet
SO mm x SO mm x
3 mm m.s. angle
SO mm x SO mm x
3 mm m.s. strip
2 mm m.s. sheet
- 52 -
each 2 430 mm
each 2 430 mm
3 pieces each
2 480 mm x
2 398 mm long
2 398 mm long
2 448 mm x
Cover sectors 2 mm m.s. sheet 2 pieces,
steam ports 50 mm x 3 mm m.s. 4 pieces,
strip each 630 mm
Lifting handles 10 mm diameter
m.s . rod
steam port covers (4 per kiln)
Bodies Either 50 mm x
3 mm m.s. strip
OR 140 mm
pipe. (Use pipe
each 500 mm
each 440 mm
OR 4 rings,
each 50 mm
Base channels (8 per kiln)
-3 mm m.s. sheet
5 mm diameter
3 mm m.s. sheet
Either 3 mm m.s.
- 53 -
4 discs, each
each 180 mm
each 500 mm x
375 x 150 mm
Smoke stacks (4 per kiln)
120 mm diameter
each 150 mm
Thin-walled steel 4 pieces,
pipe each 2 300 mm
This list may be used by the prospective charcoal-maker
as guide to determine his own investment costs according to
the domestic metal prices and to find out about the
maintenance costs of local shops.
For the filling of sacks the use of a sieve chute is
very practical. The chute is positioned in a sloped manner
and should have a width on the upper end of 1.000 mm and on
the lower side 300 mm to ke e p the sacks wide open.
The screen can be made from square wire mesh and the
mesh sizes may vary between 10 and 40 mm to separate the
charcoal f i ne s . The classification of charcoal for exports,
however , will require sieving by standardised screens .
2.2.5 The Carborion Kiln
Although the manufacturer of this type of kiln ceased a
few years after the Second World War, it is worth mentioning
for its originality. As far as is known, it is the only
portable kiln which produces charcoal in a retort with
external heating, and it may be useful to describe its
The Carborien Kiln consists of a tank of thick sheet
metal which takes the wood to be carbonized. The bottom of
the tank is perforated and it is fitted with an air-tight
lid. There are models of one-half and one stere capacity
respectively (see Figure 18).
1 = Sections of kiln shell
3 =Apertures in retort base
, = Brick bed
5 = Door in outer casing
Figure 18 The Carborion kiln
- 55 -
The tank rests on a small layer of bricks, and the whole
is enclosed in a sheet metal casing of fitted sections which
are easily dismantled. The free space between the brick
layers serves as a furnace fed through two apertures in the
When the apparatus is sited and loaded, the fire is l i t
under the retort. As soon as combust ible gases are given off
by the distillation of the wood, they must necessarily
escape through the apertures in the base of the retort. In
contact with the fire, the gases explode and so ensure
There are small sight-holes in the outer casing, so that
the ca rbonization can be followed: it is considered to be
finished when gases are no longer given off. The outer
casing is then removed, the retort is laid on the ground,
and earth is packed around its base so that air cannot enter
the retort through the apertures. The outer casing can
therefore be used with another retort.
The whole apparatus weighs 450 kg 012 stere model) or
590 kg (1 stere model).
The carbonizing period var ies from 1-1/2 hours (1/2
stere) to 4 hours 0 stere) according to the size of the
kiln and to the properties of 'wood being carbonized.
2.3 Concrete and Brick Kilns
In this category one finds the most effective kilns,
provided that they are properly constructed and operated.
Some types have proved their economic viability over more
than fifty years. The number of these kilns in operation at
present can hardly be estimated, but it is certainly close
The kiln design is simple, the investment capital requirements
are low, and a surprisingly good quality of charcoal
is produced both for household fuel and industrial uses.
Both concrete and brick types must comply with a number
of important requirements to be succesful. The kiln must be
simple to construct, relatively unaffected by thermal
stresses on heating and cooling, and strong enough to
withstand the mechanical stresses of loading and unloading.
It must be unaffected by rain and weather over six to ten
The kiln must permit control of the entry of air at all
times, and for the cooling phase there has to be a provision
for effective hermetic sealing. It must be of reasonably
lightweight construction to allow cool ing to take place
fairly easily and yet provide good thermal insulation for
the wood undergoing carbonization, otherwise the origination
of cold spots due to wind impact on the kiln walls will
prevent proper burning of the charcoal and lead to excessive
production of partially carbonized wood (brands) and low
yields. The ability of the brick kiln to conserve the heat
of carbonization is an important factor in its high
conversion efficiency of wood to charcoal .
The design of these kilns has been refined over a long
period of time. ' They can be differentiated by their shape
into hangar kilns (rectangular of square shape) and round
Hangar kilns: Missouri
kiln, Ottelinska furnace,
Round brick kilns: Argentine kiln (hal f-orange) ,
Brazilian kiln (beehive), Schwartz furnace.
The Missouri, Cinder-block, Argentine and Brazilian kilns
burn part of the charged wood within the kiln to carbonize
the remainder. The Ottelinska, Reichenbach and Schwartz
furnaces use the hot flue gases from a central fire grate,
passed through the kiln to supply heat for drying and
heating the wood to start carbonization. The Ottelinska,
- 57 -
- 58 -
u .... s,
..cC..:.:Il .... o
. ~ ....
IIIIIIIUI II 1111 1m
Schwartz and Reichenbach types require considerable amounts
of steel for buckstays on the kiln chamber, and steel grates
and doors for the furnace. Their yields (when the firewood
is counted) are not in practice superior to the others. The
Missouri kiln is well proven, it has been developed in
practice, and is still in use in the United States. It is
usually made of reinforced concrete or concrete breeze
blocks and has steel chimneys and doors. Its yield is
similar to the Argentine and Brazilian furnace. It is fitted
with large steel doors which allow mechanical equipment to
be used for loading and unloading. It has two disadvantages
for developing world use : it requires a lot of steel and
cement for its construction (both are costly, and are
usually imported items), and it is not so easy to cool as
other furnaces. It is thus more sui ted for use in temperate
climates where the materials and skills for steel and
reinforced concrete construction are at hand and low air
temperatures permit easy cooling. It is attractive where
labour, front-end loaders etc ., are readily available .
2.3.1 The Missouri Kiln
The footing for the Missouri charcoal kiln consists of
concrete, steel reinforced, 45 cm wide in front and rear and
40 cm wide at the sides . Two 1,3 cm rods are located 15 cm
from the bottom of the footing and 15 cm from each side. The
footing should be located in undisturbed soil (not in a
filled-in area) . Should the kiln be constructed in a
filled-in area , special consideration must be given to the
footing to avoid foundation failure in the future . The
footing and floor may be made of native washed sand and
gravel, as they are not required to withstand high
temperatures (see Figures 19 - 20) .
A notch is provided in the top of the footing to assist
in locking the wall to the footing. Reinforcing rods
(1,3 cm) are placed vertically 30 cm apart around the
- 60 -
foundation where the wall JOlns the footing. These rods
should extend 25 cm into the footing and have a 12 cm leg at
a 90 degree angle to ensure a strong bond (14).
The floor is a 10 cm concrete slab with 15 x 15 cm
# 10/# 10 steel reinforcing mesh. The floor has a crown down
the centre line of the kiln and at the low or drain end of
the kiln the floor slopes 15 cm to either side so that the
liquors processed from the wood will drain out of the 6 cm
pipes built in the footing. Any fill under the floor should
be of gravel packed over wetted soil to ensure a firm base.
Undesired air entrances are sealed with clay, mud or
ashes. Doors at each end of the kiln provide uninterrupted
loading and unloading of the kilns when more than one kiln
is being operated.
Construction details (14)
Six 1,50 m length of used boiler flue pipe, 10 cm in
diameter, are required for the six air inlet holes in side
walls. Four pieces of 4 m long, 10 cm diameter boiler tubes
are desirable to pipe air from the doors to near the centre
of the kiln during burning. Seven caps are required for the
seven fresh air ventilation holes made from truck rims.
Eight chimney caps are required to plug the chimneys during
the cooling phase. Two door stops are necessary for the
holes provided in the footing.
A suggested ladder and catwalk are indicated in the
figure. These provide ready access to the top of the kiln . A
ladder may be used to reach chimney tops for capping and
The volume of this kiln design is 180 m3. However, it
is expected that only 165 m3 of wood would be loaded into
it for burning.
The walls and roof are made of expanded shale aggregate
which has the same coefficient of expansion as the Portland
cement with air entraining agent. This will minimize cracks
in the kiln under the temperatures encountered in
charcoaling. Some cracks are to be expected due to the
different coefficient of expansion of the steel and
concrete. The air entraining agents cause minute air bubbles
in the concrete, and among other things, make the concrete a
better insulator which helps prevent loss of heat during the
The front and rear walls are 30 cm thick. The side walls
are 25 cm thick. This thickness provides heavy duty
unloading abuses. These abuses are, for example: throwing
the cordwood into the kiln during loading and often hitting
the wall, mechanical equipment ramming the wall, an
automoti ve truck bumping into the walls whilst loading the
Bent plates (19 mm thick) topped together with a 30 cm
I-beam on its side form the door facing for kiln protection.
Each side wall contains four 15 cm diameter tiles for
chimney entrances. A 12 cm air inlet hole is located
half-way between each chimney.
15 mm diameter reinforcing steel rods are located 30 cm
apart and centred in the walls and roof. Each intersection
is tied together with wire for additional strength.
The roof contains seven ventilation holes for fresh air
dur ing unloading of the kiln. Three of these are down the
top centre line of the kiln and two are on either side.
Their exact location may be varied within limits. To reduce
expense, these holes may be made from used truck rims cut in
half to make two forms from each rim.
Doors are large enough to provide truck and tractor
entrance for loading and unloading . The doors for the kiln
are made of 9 mm thick steel plate, 1. 50 m wide and 2.50 m
high. There are two doors closing at the centre of each end
of the kiln. Each door is hung on four 40 cm heavy duty
hinges . Fifteen 2 cm bolts are used to secure the door tight
on each end of the kiln. These bolts are spaced about 30 cm
apart on the top .
- 62 -
Photo 3 A Missouri kiln. The shell is dangerously
cracked as a result of faulty operation.
Ghana. (Photo W. Emrich)
Photo 4 Side view of kiln with two smoke pipes
and air inlet holes at the bottom. Ghana.
(Photo W. Emrich)
- 63 -
A crew of two men is needed for loading and unloading
equipment with a front-end loader and truck . One operator
per shift is sufficient to control the burning and one man
per shift can supervise a number of kilns.
The burn ing of the kiln is controlled in a similar way
to the portable metal kiln. The gas circulation system is
similar. Yields are usually better because the better
thermal insulation and greater ratio of volume to surface
area means that the endothermal heat of carbonization is
better utilized and the kiln is not so much subject to the
cooling effects of winds and rain as the un insulated metal
Missouri kilns are usually equipped with thermocouples
to read the temperature at several points within the kiln.
This is important with such large kilns as it enables cold
and hot spots to be readily detected and corrective action
taken by the operator by closing or opening air vents along
the base of the kiln. The cooling process can also be
checked so that the kiln is opened only when the t empe r a t ur e
of the charcoal is low enough'. This avoids fires which, in
such large kilns, are not easy to control even with
The sudden entry of large amounts of air into a burning
kiln may cause an explosion. Numerous minor explosions have
been reported in Missouri with no personal injuries. The
most serious explosion reported was the partial destruction
of a kiln. The top was blown off. The person closest to the
kiln was 300 m away.
It is commonly reported that kilns "puff", and lids on
air ventilation holes in the top are blown off. Such
occurrences can be avoided by proper sealing with clay or
soil, preventing the sudden entry of air, as mentioned above.
The photos 3 and 4 exhibit a not so rare damage of the
kiln shell caused by failure of the construction material
and faulty operation.
The kiln cycle is usually about 25 to 30 days, depending
on cooling rates. The capacity of two 180 m3 kilns is
about equal in wood consumption to a standard battery of
seven medium-size Brazilian kilns. But because the cycle
time is different, the utilization of labour is not so
efficient as it could be unless there are more than two
kilns to a battery. Utilization of mechanical equipment is
not optimized unless the number of kilns is sufficient to
keep it working more or less continuously.
The cycle time of a Missouri kiln in a warm climate can
be at least one month, made up as follows:
2 days 2 men plus machines.
6 days 2 men on 12 hr. or 3 men on 8 hr. shift.
20 days (min) 1 man part-time supervision.
2 days 2 men plus machines.
The total time is 30 days . If machines are not
available, the cycle time can stretch to two months or more.
The Missouri kiln's greatest advantage compared with
brick kilns is the possibility, in fact the necessity, of
mechanical loading and unloading.
Its disadvantages are the high cost, due to the use 0 f
large quanti ties of steel and concrete, and its immobility.
Unlike brick kilns, it cannot be demolished and rebuilt.
Hence a ten-year wood supply must be available within
economic haul distance of any group of kilns. The amount of
wood for a group of three 180 m3 kilns would be
60.000 m3 approximately . About 2.000 ha of forest capable
of yielding 30 m3 per hectare would have to be set aside
for ten years to supply this amount of wood. Such an area
would give a mean haulage distance of about 1 km which is
It is the belief of FAO/Rome that Missouri kilns are not
suitable for technology transfer to developing countries because
they require large quantities of costly imported items
like cement and steel. Also the long cooling time presents a
drawback which becomes sensitive in areas with a hot climate.
- 65 -
2.3.2 Cinder-Block Kilns
The masonry-type walls of these kilns should be
supported by a continous perimeter-type reinforced concrete
footing. The footing should extend at least 25 em below the
surface of well-drained ground. If only intermittent winter
operation is planned in areas where the ground freezes, the
footing should extend below the frostline. If continous
winter operation is planned or if frost seldom or never
occurs, a minimum footing depth 0 f 25 em may be used (see
Figures 21 - 22).
It is very important that the first course of blocks be
carefully laid in a full bed of mortar. If the base and
second courses are accurately laid, the balance of the
blocks will go into place with all joints perfectly broken.
All blocks are laid with the hollow cores vertical. If
hol low core blocks are used in the top course, all cores
must be filled with mortar to prevent channelling of air
into the kiln through cracks that might develop on the inner
wall surface (15).
Neat cement or the standard 1: 3 mix of cement and sand
may be used to level of f the tops of the front wall blocks
over which the bottom of the angle-iron lintel must rest in
order to seal off the ceiling cover with sand . A piece of
bright sheet metal may also be used between the angle lintel
and the top of the wall to permit the lintel to slide more
easily along the top of the wall. A loose brick may be used
to retain the sand at the end of the lintel .
One or two courses of brick are commonly laid around the
top edge of the kiln to act as a coping. The purpose of the
coping is to help prevent the ceiling sand from being washed
and blown off the ceiling steel. Sections of steel rails or
I-beams can serve both as a coping material and as a support
for the ceiling beams. They also distribute the weight of
the ceiling beams along the s ide walls and restrain the
walls from bowing outwards at the top .
~ .... U
..... .C..I.J CIJ
·S :J u 0 l.>
Good workmanship is very important when laying the
walls. If an experienced mason is not available, some good
manual of recommended practices should be consul ted before
attempting to lay any block. Such publications will provide
dimensions of the various types of blocks, recommended
mortar mixes, and many helpful suggestions for building a
All mortar joints must be carefully compressed and left
neat and compact, either in a concave or V-shape. Such
joints will provide a good valley for sealing compound as
sealing becomes necessary during operation. Other types of
mortar joints are not recommended.
Either one or as many as four chimneys are normally
used. When only one chimney is used, it is located in the
centre of the rear wall. When three chimneys are used,
another is added at the lengthwise centre of each side wall.
When four are used, one is placed at or near each of the
corners of the kiln.
15 or 25 em diameter sheet-metal chimneys are supported
on loose resting on masonry blocks. Chimney bases are
constructed from loose pier-type masonry blocks placed
directly on the ground, with loose steel plate covers
resting on the blocks. Two 1.0 by 40 by 50 em plates are
used at each chimney. One plate next to the kiln is Left
loose and removable so that a shovelful of sand can be added
for closing-off the chimney during the cooling period.
Partial or full-length insulation of metal-type chimneys
is helpful in colder climates to retard the condensation and
build-up of tars. Chimney tile has been used success fully
inside masonry block chimneys, particularly those partially
or wholly buried in an earth fill. Some commercial chimneys
have been made from concrete masonry block without any
lining. All chimneys should extend at least 30 cm above the
top of the kiln structure.
Front-entry air supply has given satis fatory results in
both one- and three-chimney designs. Front air entry is most
easily obtained by hanging the sliding metal door so that